- Nano Express
- Open Access
Toward Exploring the Structure of Monolayer to Few-layer TaS2 by Efficient Ultrasound-free Exfoliation
Nanoscale Research Letters volume 13, Article number: 20 (2018)
Tantalum disulfide nanosheets have attracted great interest due to its electronic properties and device applications. Traditional solution-ased ultrasonic process is limited by ultrasound which may cause the disintegration into submicron-sized flake. Here, an efficient multi-step intercalation and ultrasound-free process has been successfully used to exfoliate 1T-TaS2. The obtained TaS2 nanosheets reveal an average thickness of 3 nm and several micrometers in size. The formation of few-layer TaS2 nanosheets as well as monolayer TaS2 sheets is further confirmed by atomic force microscopy images. The few-layer TaS2 nanosheets remain the 1T structure, whereas monolayer TaS2 sheets show lattice distortion and may adopt the 1H-like structure with trigonal prism coordination.
Layered transition metal dichalcogenides (TMDs) have attracted great interest as two-dimensional materials due to their unique structural features and outstanding performances in the field of energy [1,2,3,4,5,6,7,8,9] and electricity [10,11,12,13,14]. Because of their lamellar structures, TMDs usually serve as the hosts for the intercalation of a wide variety of electron-donating species ranging from Lewis bases to alkali metals and can be exfoliated into nanosheets using organolithium  or alkali metal naphthalene  reduction chemistry and ultrasound physics [5, 9, 11, 15,16,17,18,19]. The exfoliated TMDs usually show enhanced properties in the field of electric [11, 14], catalyst [5, 6, 8, 9], and energy storage [2,3,4, 7].
As one of the typical TMD isomorphism, tantalum disulfide (TaS2) shows a unique combination of valuable structural, mechanical, chemical, and electronic properties, which has been studied for decades [10, 12, 15, 20,21,22]. Its lamellar structure and electronic properties are beneficial for high-power applications such as micro-electromechanical system, device applications [18, 21, 23], and superconductor [10, 12]. 1T and 2H phases are the most representative structures. The distinction between two phases can be the S-Ta-S coordinated situations, which are recognized as octahedral coordination (1T) and prismatic coordination (2H). The two phases are quite different in electronic structures and other properties. For example, bulk 1T-TaS2 shows charge density wave (CDW) transition and such a transition is found to vanish measured at (001) oriented single-crystal nanoflake (< 5 nm thickness) [18, 21, 23]. Whereas, the 2H phase shows superconductivity and its critical temperature can be raised by intercalation [24,25,26].
TMDs including TaS2 can be successfully exfoliated by mechanical method  or ultrasound-assisted intercalation process [1, 4,5,6,7,8,9, 14, 15, 19]. The exfoliated TaS2 obtained by mechanical method is only used to explore its microscopic properties [20, 23, 27]. All the other methods have not got rid of the physical ultrasound assistance [15,16,17, 19], which may suffer the size of the exfoliated nanoflakes  and limits their wide applications. Therefore, it is necessary for us to explore an efficient alternative exfoliation route.
Our search leads us to a multi-step intercalation method using alkali metal-ammonia as the first step intercalation reaction. In sodium liquid ammonia solution, for example, the metal transfers an electron to the solution to produce a radical solvated electron. The reaction introduces both alkali metal and ammonia molecule into the interlayer of TaS2. Moreover, the ammonia can be replaced by hydroxyl-contained water . Hydroxyl-contained glucose was ever used to intercalate perovskite [29, 30] which can produce very large layer spacing. It is interesting to consider whether the hydroxyl-contained glucose can get into the TaS2 layer just like water and achieve the exfoliation of TaS2. And water-organic mixed solvent was ever employed to exfoliate high-quantity two-dimensional material [31, 32].
Herein, using a multi-step ultrasound-free intercalation process, we report efficient exfoliation of 1T-TaS2. The exfoliated TaS2 nanosheets show 1T structure with several micrometers in size and an average thickness of about 3 nm. Monolayer TaS2 can also be obtained, and some work was done to explore its structure features.
Ta, Na, and S power are available from Aladdin reagent. All reagents were used as received without further purification.
First, 1T-TaS2 was prepared by sealing a stoichiometric amount of Ta and S in vacuum quartz tube, then quenching the tube after heating to 900 °C for 1 day.
The exfoliation mechanism can be attributed to a multi-step intercalation process. Na x (NH3) y TaS2 was synthesized through liquid ammonia procedure. First, a sealed reaction bulb with certain amounts of sodium was placed under − 80 °C to obtain the ammonia solution of sodium. Then, the TaS2 powder was added into the deep-blue solution with a molar ratio of TaS2:Na being 1:0.8. After a 10–20-min reaction, liquid ammonia evaporated and Na x (NH3) y TaS2 was available.
Fifty milligrams of Na x (NH3) y TaS2 was exposed in air to transfer to Na x (H2O) y TaS2, after this, the Na x (H2O) y TaS2 was ground and added to 20 ml 0.2 g/ml aqueous glucose solution. The mixing solution was stirred for 5 min to disperse in the air and then bubbled with nitrogen to expel the oxygen for avoiding the oxidation. Na x (C6H12O6) y TaS2 can be separated from the reaction solution after about 2 h. The above dispersion was sealed and kept stirring for 6 h. Then, the solution was centrifuged at 12000 rpm for 30 min to obtain the product (marked as sample A) for further characterization. For contrast, part of the solution was standing for 1 h and the supernatant solution was centrifuged (marked as sample B). The water bubbled with nitrogen for more than 30 min (anaerobic water) could be utilized to wash off glucose and then alcohol was used to wash the sample to move water.
X-ray diffraction (XRD) patterns were recorded on a Philips X’pert Pro Super diffractometer with Cu Kα radiation at room temperature. XRD pattern of Na x (NH3) y TaS2 was measured in air-free capillary tube, differently, and all the other intercalated samples were measured in air. The scanning electron microscopy (SEM) images were taken on a JEOL JSM-6700F field emission scanning electron microscope (FESEM, 20 kV). Transmission electron microscopy (TEM) images were obtained on a JEOL-2010 with an accelerating voltage of 200 kV. Atomic force microscopy (AFM, DI Innova Multimode SPM platform) was used for detecting the thickness. Microscopic structure investigations were carried via high-angle annular dark field (HAADF) imaging mode in an advanced JEM-ARM 200F aberration-corrected high-resolution TEM facility.
Results and Discussion
Figure 1 shows the schematic diagram of the multi-step intercalation reactions. The alkali metal-ammonia has reducibility and can be introduced simultaneously into the 1T-TaS2 interlayer gallery to obtain Na x (NH3) y TaS2 within a short time. Na x (NH3) y TaS2 is not stable and easily transfers to Na x (H2O) y TaS2 in water, along with the de-intercalation of Na+ and the generation of hydrogen [33, 34]. After transferring Na x (H2O) y TaS2 into the aqueous glucose solution, Na x (C6H12O6) y TaS2 can form and be separated after 2 h. Then, after a total of 6 h, exfoliated TaS2 forms eventually owing to the constant de-intercalation of Na+ and the weak interaction between glucose molecule and TaS2 layer. The flame reaction of reaction solution further confirms the de-intercalation of Na+, and the reaction formulas are shown (Additional file 1: Figure S1).
It is found that full dispersal of Na x (H2O) y TaS2 in glucose solution is a key factor to exfoliate TaS2. Additional file 1: Figure S2 shows the disperse status of Na x (H2O) y TaS2 in aerobic water, i.e., operating in air, and anaerobic water, i.e., dispelling the oxygen of water, respectively. If oxygen is bubbled before adding Na x (H2O) y TaS2, it will never be dispersed in aqueous glucose solution and exfoliated TaS2 cannot be obtained. In contrary, Na x (H2O) y TaS2 can be fully dispersed in aerobic water, which may be due to the hydroxylation process of the layer edge . Then, the full dispersal leads to the effectively exfoliation. All products can be centrifuged and used for the characterization.
XRD patterns (Fig. 2a) show the interlayer spacing changes of each stage. The 001 peak of pristine TaS2 is shifted completely toward lower angles, indicating expansion of the lattice along the c-axis. The interlayer spacing of Na x (NH3) y TaS2, Na x (H2O) y TaS2, and Na x (C6H12O6) y TaS2 are 9.1, 11.7, and 14 Å, respectively. Comparing with the 5.86 Å of TaS2, the interlayer spacing of Na x (C6H12O6) y TaS2 has increased by 8.1 Å, which would greatly weaken the Van der Waals’ force of interlayer and is of advantage to the exfoliation of TaS2.
Figure 2b (A) shows the XRD pattern of sample A. The 001, 002, 100, 101, and 003 peaks are completely in accordance with 1T-TaS2. The sharp 100 peak, and wide and strong 00 l reflections indicate the ab extensional orientation of the nanosheets. The average thickness is estimated to be 3 nm by Scherrer equation based on the FWHM of 001 peak. Besides, The XRD pattern (Fig. 2b (B)) of sample B shows that the 001 peak vanishes completely, i.e., the period of c-axis disappears, meaning the formation TaS2 monolayers. Besides, as the same structure, 1T-TiS2 can also be exfoliated by our method. The XRD pattern of exfoliated TiS2 is shown in Additional file 1: Figure S3. The average thickness of exfoliated TiS2 is estimated to be 4 nm by Scherrer equation. This shows the potential of our method to expand into other TMDs.
Additional file 1: Figure S4 shows the Raman spectra of bulk TaS2 and exfoliated nanosheets. There are two Raman features that can be determined, which are E1g and A1g modes [35, 36]. From bulk to nanosheet, the E1g and A1g modes show some shifts. These shifts are probably attributed to the decrease of the force constant resulted from the weakening of the interlayer Van der Waals force between layers. There is also a new mode of vibration which may come from structure changes. The FWHM of exfoliated TaS2 is larger than that of bulk, which also indicates the decrease of thickness
The FESEM images in Fig. 3a, b clearly reveal flake-like morphology with several micrometers in size. One remarkable result is the case that most of the TaS2 sheets have micro-sized proportion. TEM images of Fig. 3c, d further show the morphology of the sample.
Figure 4 shows the AFM analysis performed on samples which are deposited on muscovite substrate. We measured three sheets (0.45, 0.45, and 2.1 nm, respectively). The thickness of 0.45 nm is within the permissible range of the 001 interlayer spacing of 5.86 Å, and the polyhedron size of 2.93 Å formed by Ta and S atoms (more evidence can be seen in HADDF image of Additional file 1: Figure S5), which is the direct evidence of the formation of monolayer TaS2. Meanwhile, the 2.1-nm-thick nanosheet stands for three to four layers of TaS2.
Our approach can produce micro-sized sheets (maximum lateral size is 5 μm) and monolayer TaS2 (minimum thickness is 0.45 nm). Ultrasound is not necessary and may suffer the size of the exfoliated nanoflakes. More details about the differences between different exfoliation techniques are shown in Additional file 1: Table S1.
Figure 5 displays the high-resolution transmission electron microscopy (HRTEM) image and fast Fourier transformation (FFT) patterns of a crisscross structure. The lattice fringes of 2.9 and 5.9 Å are consistent with 100 and 001 planes of bulk TaS2, respectively. FFT patterns were carried on the typical  zone axis (A) and / zone axis (B), respectively. In addition to the overlapping part, 101 and 001 diffraction spots of 1T-TaS2 on B region are identified, indicating that the few-layer nanosheets adopt 1T-TaS2 structure.
We also carried out atomic structure investigations via HAADF imaging mode in an advanced aberration-corrected high-resolution STEM facility. Figure 6a recorded at a few-layer TaS2 sheet shows a 1T atomic structure which can be clearly seen in the HAADF image. The distance between two Ta atoms is 3.35 Å, and the FFT pattern shows the normal 2.9 Å spot of 100. To further explore the structure, we have utilized the Z-contrast in HAADF-STEM images (Fig. 6a). The contrasts contributed by S atoms distribute symmetrically along the AB line (Fig. 6c). The results are consistent with the octahedral coordination of S-Ta-S in 1T-TaS2 structure (Additional file 1: Figure S6a) . S atoms are symmetrically distributed around the Ta sites (Fig. 6c).
When we further characterized the monolayer nanosheet, an interesting phenomenon is found that the atomic distance between two Ta atoms from three directions are 3.4, 3.45, and 3.53 Å, respectively (Fig. 6b). The corresponding FFT pattern shows a distorted hexagon (2.93, 2.98, and 3.07 Å, respectively) which indicates the lattice distort in ab plane (Fig. 6b). The intensity profile recorded along CD line (Fig. 6e) differs from the case of few-layer TaS2 (Fig. 6c). The contrasts contributed by S atoms distribute asymmetrically along the CD line, and its relative intensities are much stronger than that in Fig. 6c, which means another S-Ta-S coordination in the monolayer structure. Note that there are two S-Ta-S coordinated situations in TaS2, the results are consistent with the 1H single layer structure with trigonal prism coordination of S-Ta-S (Additional file 1: Figure S6b) . In this case, the S atoms are asymmetrically distributed around Ta atom along the CD line, and the overlap of two S atoms along c-axis (the electron beam direction) result in the enhancement of the signal from the S atoms (Fig. 6f). Therefore, 1H structure with trigonal prism coordination of S-Ta-S in monolayer TaS2 sheet is proposed. Such a single layer structure may be unstable, and the lattice distortion would probably occur. This structure may be responsible for the new vibration mode in Raman result. Of course, the essence of lattice distortion in monolayer TaS2 should be further explored. Meanwhile, different structural phases of TaS2 sheets may be exploited for different device applications.
In summary, we have developed an efficient exfoliation method for the exfoliation of tantalum disulfide and obtained micron-sized monolayer to few-layer sheet. This is a pure chemical exfoliation method in which ultrasound is not necessary. Monolayer and few-layer sample have all been characterized in detail, and coordination change from octahedron to triangular prism is found on monolayer TaS2. This really warns everyone to pay attention to the point of property variation caused by structural changes in exploring the finite-size effect, while few-layer TaS2 still keeps the 1T structure.
Briefly, the present work not only provides an efficient ultrasound-free strategy for synthesizing high-exfoliated functional nanosheets but also explores the structure of monolayer and few-layer TaS2. The present work will provide insights to better understanding 2D materials and their physical and chemical properties, and offer more opportunities for their applications.
Voiry D, Yamaguchi H, Li J, Silva R, Alves DC, Fujita T, Chen M, Asefa T, Shenoy VB, Eda G, Chhowalla M (2013) Enhanced catalytic activity in strained chemically exfoliated WS2 nanosheets for hydrogen evolution. Nat Mater 12:850–855
Feng J, Sun X, Wu C, Peng L, Lin C, Hu S, Yang J, Xie Y (2011) Metallic few-layered VS2 ultrathin nanosheets: high two-dimensional conductivity for in-plane supercapacitors. J Am Chem Soc 133:17832–17838
Li H, Shi Y, Chiu M-H and Li L-J 2015. Emerging energy applications of two-dimensional layered transition metal dichalcogenides. Nano Energy 18:293-305
Li Y, Liang Y, Robles Hernandez FC, Deog Yoo H, An Q, Yao Y (2015) Enhancing sodium-ion battery performance with interlayer-expanded MoS2–PEO nanocomposites. Nano Energy 15:453–461
Lukowski MA, Daniel AS, Meng F, Forticaux A, Li L, Jin S (2013) Enhanced hydrogen evolution catalysis from chemically exfoliated metallic MoS2 nanosheets. J Am Chem Soc 135:10274–10277
Mahler B, Hoepfner V, Liao K, Ozin GA (2014) Colloidal synthesis of 1T-WS2 and 2H-WS2 nanosheets: applications for photocatalytic hydrogen evolution. J Am Chem Soc 136:14121–14127
Muharrem Acerce DV, Manish Chhowalla* (2015) Metallic 1T phase MoS2 nanosheets as supercapacitor electrode materials. Nat Nanotechnol 10:313–318
Nguyen TP, Choi S, Jeon J-M, Kwon KC, Jang HW, Kim SY (2016) Transition metal disulfide nanosheets synthesized by facile sonication method for the hydrogen evolution reaction. J Phys Chem C 120:3929–3935
Sun X, Dai J, Guo Y, Wu C, Hu F, Zhao J, Zeng X, Xie Y (2014) Semimetallic molybdenum disulfide ultrathin nanosheets as an efficient electrocatalyst for hydrogen evolution. Nano 6:8359–8367
Ang R, Tanaka Y, Ieki E, Nakayama K, Sato T, Li LJ, Lu WJ, Sun YP, Takahashi T (2012) Real-space coexistence of the melted Mott state and superconductivity in Fe-substituted 1T-TaS2. Phys Rev Lett 109:176403
Feng J, Peng L, Wu C, Sun X, Hu S, Lin C, Dai J, Yang J, Xie Y (2012) Giant moisture responsiveness of VS2 ultrathin nanosheets for novel touchless positioning interface. Adv Mater 24:1969–1974
Sipos B, Kusmartseva AF, Akrap A, Berger H, Forro L, Tutis E (2008) From Mott state to superconductivity in 1T-TaS2. Nat Mater 7:960–965
Taniguchi K, Matsumoto A, Shimotani H, Takagi H (2012) Electric-field-induced superconductivity at 9.4 K in a layered transition metal disulphide MoS2. Appl Phys Lett 101:042603
Lin C, Zhu X, Feng J, Wu C, Hu S, Peng J, Guo Y, Peng L, Zhao J, Huang J, Yang J, Xie Y (2013) Hydrogen-incorporated TiS2 ultrathin nanosheets with ultrahigh conductivity for stamp-transferrable electrodes. J Am Chem Soc 135:5144–5151
Zheng J, Zhang H, Dong S, Liu Y, Nai CT, Shin HS, Jeong HY, Liu B, Loh KP (2014) High yield exfoliation of two-dimensional chalcogenides using sodium naphthalenide. Nat Commun 5:2995
Bang GS, Cho S, Son N, Shim GW, Cho BK, Choi SY (2016) DNA-assisted exfoliation of tungsten dichalcogenides and their antibacterial effect. ACS Appl Mater Interfaces 8:1943–1950
Guan G, Zhang S, Liu S, Cai Y, Low M, Teng CP, Phang IY, Cheng Y, Duei KL, Srinivasan BM, Zheng Y, Zhang YW, Han MY (2015) Protein induces layer-by-layer exfoliation of transition metal dichalcogenides. J Am Chem Soc 137:6152–6155
Hengcong Tao YZ, Gao Y, Sun Z, Yan C, Texter J (2017) Scalable exfoliation and dispersion of two-dimensional materials––an update. Phys Chem Chem Phys 19:921–960
Jawaid A, Nepal D, Park K, Jespersen M, Qualley A, Mirau P, Drummy LF, Vaia RA (2016) Mechanism for liquid phase exfoliation of MoS2. Chem Mater 28:337–348
Tsen AW, Hovden R, Wang D, Kim YD, Okamoto J, Spoth KA, Liu Y, Lu W, Sun Y, Hone JC, Kourkoutis LF, Kim P, Pasupathy AN (2015) Structure and control of charge density waves in two-dimensional 1T-TaS2. PNAS 112:15054–15059
Wang L, Kanatzidis MG (2001) Laminated TaS2/polymer nanocomposites through encapsulative precipitation of exfoliated layers. Chem Mater 13:3717–3727
Ma L, Ye C, Yu Y, Lu XF, Niu X, Kim S, Feng D, Tomanek D, Son YW, Chen XH, Zhang Y (2016) A metallic mosaic phase and the origin of Mott-insulating state in 1T-TaS2. Nat Commun 7:10956
Yoshida M, Zhang Y, Ye J, Suzuki R, Imai Y, Kimura S, Fujiwara A, Iwasa Y (2014) Controlling charge-density-wave states in nano-thick crystals of 1T-TaS2. Sci Rep 4:7302
Fang L, Wang Y, Zou PY, Tang L, Xu Z, Chen H, Dong C, Shan L, Wen HH (2005) Fabrication and superconductivity of NaxTaS2 crystals. Phys Rev B 72: 014534
Li LJ, Zhu XD, Sun YP, Lei HC, Wang BS, Zhang SB, Zhu XB, Yang ZR, Song WH (2010) Superconductivity of Ni-doping 2H–TaS2. Physica C Supercond 470:313–317
Biberacher W, Lerf A, Besenhard JO, Möhwald H, Butz T, Saibene S (1983) Electrointercalation into 2H-TaS2 single crystals: in situ dilatometry and superconducting properties. Il Nuovo Cimento 2D:1706–1711
Yu Y, Yang F, Lu XF, Yan YJ, Cho YH, Ma L, Niu X, Kim S, Son YW, Feng D, Li S, Cheong SW, Chen XH, Zhang Y (2015) Gate-tunable phase transitions in thin flakes of 1T-TaS2. Nat Nanotechnol 10:270–276
Levy F (1979) Intercalated layered materials. Phys Chem Mater Layered Struct 6:159–169
Wang C, Tang K, Wang D, Liu Z, Wang L (2012) Simple self-assembly of HLaNb2O7 nanosheets and Ag nanoparticles/clusters and their catalytic properties. J Mater Chem 22:22929
Wang C, Tang K, Wang D, Liu Z, Wang L, Zhu Y, Qian Y (2012) A new carbon intercalated compound of Dion–Jacobson phase HLaNb2O7. J Mater Chem 22:11086
Manna K, Huang HN, Li WT, Ho YH, Chiang WH (2016) Toward understanding the efficient exfoliation of layered materials by water-assisted cosolvent liquid-phase exfoliation. Chem Mater 28:7586–7593
Manna K, Hsieh CY, Lo SC, Li YS, Huang HN, Chiang WH (2016) Graphene and graphene-analogue nanosheets produced by efficient water-assisted liquid exfoliation of layered materials. Carbon 105:551–555
Bratsch SG (1989) Standard electrode potentials and temperature coefficients in water at 298.15K. J Phys Chem Ref Data 18:1–22
Oh DY, Choi YE, Kim DH, Lee YG, Kim BS, Park J, Sohn H, Jung YS (2016) All-solid-state lithium-ion batteries with TiS2 nanosheets and sulphide solid electrolytes. J Mater Chem A 4:10329–10335
Hirata T, Ohuchi FS (2001) Temperature dependence of the Raman spectra of 1T-TaS2. Solid State Commun 117:361–364
Wu MH, Zhan J, Wu K, Li Z, Wang L, Geng BJ, Wang LJ, Pan DY (2017) Metallic 1T MoS2 nanosheet arrays vertically grown on activated carbon fiber cloth for enhanced Li-ion storage performance. J Mater Chem A 5:14061–14069
Liu Q, Li X, Xiao Z, Zhou Y, Chen H, Khalil A, Xiang T, Xu J, Chu W, Wu X, Yang J, Wang C, Xiong Y, Jin C, Ajayan PM, Song L (2015) Stable metallic 1T-WS2 nanoribbons intercalated with ammonia ions: the correlation between structure and electrical/optical properties. Adv Mater 27:4837–4844
Voiry D, Mohite A, Chhowalla M (2015) Phase engineering of transition metal dichalcogenides. Chem Soc Rev 44:2702–2712
This work was supported by the National Natural Science Foundation of China (no. 21671182).
National Natural Science Foundation of China (no. 21671182).
Availability of Data and Materials
All data are fully available without restriction.
The authors declare that they have no competing interests.
Springer Nature remains neutral with regard to jurisdictional claims in published maps and institutional affiliations.
About this article
Cite this article
Hu, Y., Hao, Q., Zhu, B. et al. Toward Exploring the Structure of Monolayer to Few-layer TaS2 by Efficient Ultrasound-free Exfoliation. Nanoscale Res Lett 13, 20 (2018). https://doi.org/10.1186/s11671-018-2439-z
- Tantalum disulfide
- Layer material
- Structural transition